4. Henry, C.H., Schnatterly, S.E. and Slichter, C.P., Phys. Rev. A 137, 583 (1965).
5. Mackey, D.J., Runciman, W.A. and Vance, E.R. Phys. Rev. B 11, 211 (1975) .
Zeeman studies of band-edge excitons in Pb^. 4.1.1. Introduction
4.1.2. Exciton theory applicable to P b ^ 4.1.3. Growth of single crystals
4.1.4. Experimental results
4.1.5. Comparison with other experimental data
4.1.6. Discussion of studies critical of the single hydrogenic series
4.1. Zeeman studies of band-edge excitons in P b ^ 4.1.1. Introduction
Lead iodide is an anisotropic semiconductor and it crystallizes
in the hexagonal cadmium iodide-like structure (space group D ^ ) . Layers of lead and iodine atoms lie perpendicularly to the c axis. The sequence of the layers is repeated in units of I-Pb-I and the layers are held
together by Van der Waal forces . Lead iodide is known to exhibit 3
structural polytypism , where the 2H, 4H, 6R.... polytypes describe various stacking arrangements of the basic I-Pb-I layer. The different polytypes are classified by the number of I-ion layers within the unit repeat distance along the c axis followed by the letter H or R; for hexagonal or rhombo- hedral polytypes.
Nikitine and Perny^ observed a series of lines in the low tempera ture absorption spectrum of single crystals of lead iodide, on the long wavelength side of the fundamental absorption edge, at '''20,000 cm . These lines were assigned to a three-dimensional hydrogenic exciton series, whose energies could be represented by
vn = 20,711 - n = 2,3,4 . (4-1)
The n=l line was observed ~650 cm ^ higher in energy from the position given by eq. 4-1.
Some reservations about the existence of a hydrogenic exciton series in lead iodide must be mentioned, since some investigators suggest that the n=l, n=2 and n=3 lines do not belong to a single hydrogenic series. Alternative explanations have been given to account for these lines which are all in contradiction with the conclusions of Nikitine and Perny.
This investigation was initiated to study these excitons in single crystals of lead iodide. The principal experimental investigation involved
MCD studies of the n=l, n=2 and n=3 lines. The only previous MCD study has been reported by Baldini and Franchif’, who worked with thin films and observed only the n=l line. In addition, for the first time, these excitons were studied in a high magnetic field of 21T.
4.1.2. Exciton Theory Applicable to Lead Iodide
The concept of an exciton has been introduced by Frenkel^* to explain the mechanism by which pure insulating solids absorb electro magnetic radiation. He suggested that electrons in solids could exist in bound excited states similar to atomic excited states, and that these bound states can move through the crystal by a hopping mechanism.
Alternatively, Wannier visualised an exciton as an electron in the conduction band coupled by Coulomb interaction to a hole in the valence band, the electron-hole combination being free to move through the crystal. The Wannier picture can be taken over to the Frenkel picture, and physically
they differ only in the electron-hole separation ; the Wannier model applies to excitons for which the electron-hole separation is larger than the lattice constant, whereas, for the Frenkel model, the electron-hole separation is smaller than the lattice constant. For the Wannier model, which is relevant to this discussion, the Coulomb interaction between the electron and the
hole is modified by the medium, and given by -— , where e is the dielectric constant of the medium.
The theoretical description of the Wannier excitons has been
developed amongst others by Dresselhaus and Elliott , in terms of the effective mass approximation. In this approximation it is assumed that the valence and conduction bands are parabolic. (In the E versus k curves, E ^ k," at the k value where the transition takes place.) Moreover, if it
is assumed that the electron and the hole have isotropic effective masses m^* and m^* respectively, then the exciton problem reduces to the three- dimensional hydrogen atom problem, where the potential energy is given by
2 6 - — , and t h e k i n e t i c e n e r g y i s g i v e n i n t e r m s o f y, t h e r e d u c e d mass o f t h e e x c i t o n :
V( 4 - 2 ) The e n e r g i e s o f t h e s e r i e s o f l i n e s n = l , 2 , 3 , . t h r e e - d i m e n s i o n a l h y d r o g e n i c e x c i t o n s p e c t r a a r e g i v e n by ^ i n t h e V = E - R / n 2 n gap n = 1 , 2 , 3 , . . ( 4 - 3 ) and t h e i n t e n s i t i e s , I , by * n * J I n n -3 n = l , 2 , 3 , . . . ( 4 - 4 )
E^ i s t h e e n e r g y gap b et wee n t h e v a l e n c e and c o n d u c t i o n b a n d s , and R, t h e e f f e c t i v e Rydberg o r t h e e x c i t o n b i n d i n g e n e r g y i s g i v e n by 4 ye 2 2 2c Fi ( 4 - 5 )
The h y d r o g en atom a p p r o x i m a t i o n i s v a l i d f o r o r b i t s o f l a r g e r a d i u s , where t h e s c r e e n e d Coulomb i n t e r a c t i o n v a r i e s s m oo t hl y by v i r t u e o f t h e f a c t t h a t £ i s a c o n s t a n t a t l a r g e d i s t a n c e s from t h e h o l e , and i s o n l y a r ough a p p r o x i m a t i o n f o r o r b i t s o f s m a l l r a d i u s .
The p r e d i c t i o n s o f t h e s i m p l e h y d r o g e n i c e x c i t o n t h e o r y have
been b o r n e o u t by t h e o b s e r v a t i o n o f l i n e s e r i e s which s a t i s f y e q u a t i o n ( 4 - 3 ) , i n t h e low t e m p e r a t u r e a b s o r p t i o n s p e c t r a o f Cu^O^ . In f a c t , N i k i t i n e ^ h a s o b s e r v e d , i n Cu^O, t h r e e s e r i e s o f l i n e s known as t h e y e l l o w , g r e e n and r e d s e r i e s . For e xa m p l e , t h e y e l l o w s e r i e s a t 4 . 2 K can be r e p r e s e n t e d by
v = 17,525 - Z M c m ' 1
n ’ 2 n = 2 , 3 , 4 , ( 4 - 6 )
N i k i t i n e has o b s e r v e d l i n e s u p t o n=6 a t 4 . 2 K, and l i n e s up t o 12
been observed ~350 cm lower in energy than given by the above formulae This lowering in energy of the n=l line has been qualitatively explained
by Haken as being due to the inapplicability of the macroscopic dielectric constant for small radius (n=l) excitons.
As mentioned earlier, for P b ^ , the n=l line was observed 6S0 cm ^ higher in energy from the position given by eq. (4-1), which is in marked contrast to the shift towards lower energy in the case of the n=l line in Cu^O. This shift towards higher energies has been explained, by Ilarbeke
15 1 6 1 7
and Tosatti , in terms of the central cell corrections * , following the observation that the excitons in Pbl„ are cationic. Studies of Pb, Cd I„
2 1-x x 2
alloys have shown that the position of the n=l line varies linearly with x between 2.497 e.v. for x=0 and 3.23 ± .01 e.v. for x=0.99. Furthermore,
Goto and Ueta have observed an absorption band at 3.24 e.v. in Pb-doped Cdl^ for x=0.999 and assigned it to an internal s-p crystal field transition of the Pb^ ion. Thus, since the n=l exciton line connects right through to the Pb^+ impurity absorption in Cdl2 , it follows that the n=l exciton must be predominantly cationic, i.e. both valence and conduction bands of Pbl^ have strong admixtures of Pb wavefunctions. The cationic nature of the excitons in Pbl^ has been confirmed by the charge density calculations of SchlUter and Schlüter^. Now, since both the electron and hole wave-
functions originate from the same sort of atom, the orthogonality requirements become very stringent and thus a repulsive central cell correction would
arise. Hermanson and Phillips , and Hermanson have shown that there are three central cell corrections to the hydrogenic model; (1) breakdown of the dielectric macroscopic screening, (2) non-parabolic energy bands, and (3) repulsive terms in the central cell. The first two effects shift the energy below the hydrogenic value, whilst the repulsive central cell correction which arises due to the non-orthogonality of the wavefunctions gives positive energy shifts. Further, Hermanson has shown for excitons
4.1.3. Growth of Single Crystals
Crystals of Pbl^ were grown both from silica gels and from aqueous solution.
Crystal growth in gels is well suited for substances such as Pbl^ which have low solubilities and therefore cannot easily be grown
from solution . Following Henisch , a solution of reagent grade sodium 3
metasilicate (having specific gravity ~1.06 gm/cm ) was mixed with a dilute solution of acetic acid in a test tube. The sodium metasilicate wns added drop by drop to the acid with constant stirring, to avoid excessive local ion concentrations which otherwise cause premature local gelling and make the final medium inhomogeneous and turbid. When the solution in the test tube reached a pH of 4 (as determined by Rota universal indicator), a small amount of IN lead acetate solution was added and the whole mixture allowed to gel at room temperature. A 0.5N solution of potassium iodide was then placed on top of the gel. Thin, yellow platelets of Pbl^ about 3 to 4 mm in diameter were obtained in two to three weeks time.
Pbl9 crystals were also grown from an aqueous solution, as follows 0.001M of basic lead acetate and an equivalent molar amount of KI were separately dissolved and heated to the boiling point in ~4% acetic acid solution. The presence of acetic acid is important, because it prevents
atmospheric oxidation and complexation of KI and Pbl9 . The solutions were then mixed intimately and small crystals of P b ^ formed on cooling. The crystals were washed and dissolved again in ~4% acetic acid solution to produce a concentrated solution of Pbl^. The solution was placed in an open dish which was floated on a water bath at 90°C. The bath was
allowed to cool slowly and the process of crystallization which takes place at the surface as well as in the bulk of the solution was observed at
frequent intervals. The crystals were extracted from the solution on
glass slides, to which they adhered without further treatment. The crystals thus obtained were not of uniform thickness, and metal masks were used
so that as far as possible only a uniform crystal thickness was visible.
4.1.4. Experimental Results
Crystals. Most of the quantitative absorption and MCD data were obtained on two crystals, the thinner being designated A1 and the thicker A 2 . Several other crystals grown from silica gels and from
solution were also investigated, but they were too thick for quantitative analysis on the n=l line, because of the very strong absorption. Satisfactory X-ray transmission Laue photographs were obtained from all these crystals except Al, and the c axis of each was perpendicular to the substrate; A2 gave the best defined Laue pattern. Al was probably too thin to give a pattern distinguishable from the diffuse scattering due to the glass backing.
Absorption. Low temperature axial absorption spectra uncorrected for reflection effects are shown in Figures (4-1) and (4-2) for crystals Al and A2 respectively. The "extra" absorption feature on the low energy
side of the n=l peak is due to reflection effects (see Nikitine et_ al_ ). Figure (4-2) also shows the temperature dependence of the absorption spectrum for crystal A2. Figure (4-3) shows the details of Figure (4-2) on an
expanded scale. The temperature dependence of the absorption spectra shown in Figures (4-2) and (4-3) was qualitatively confirmed with the thicker samples, in which the top of the absorption maxima of the n=l line was cut off by stray and scattered light.
o _cO O CD CD
Ä j j s u e Q |i?3!|dQF ig ur e ( 4 - 1 ) . Ax ia l a b s o r p t i o n sp ec tr u m f o r crystal A l .
W a v e n u m b e r (1 04 c m )
W a v e l e n g t h ( n m )
W a v e n u m b e r (1 04 c m 1)2 .0 8 2 .0 4 2.0 0 1.96
W a v e l e n g t h ( n m )
Reflection Studies. Six relatively thick crystals grown both
from gels and aqueous solution were studied at low temperatures in reflection and one such reflection spectrimis shown in Figure (4-4).